WELDERS HAND BOOK .
THE CHOICE OF A SUITABLE ELECTRODE
When Choosing an electrode, the first rule is to select one which gives a
weld metal quality equal to or better than that of the base metal . Welding
Position & type of joint are other factors, which influence the choice of
General information on the influence of the electrode coating type on
welding properties, welding speed and weld metal quality .
Rutile Electrodes giving about 100% weld metal recovery are easy to
strike and use and are particularly suitable for short welds in mild steel,
for fillet welding,welding sheet Steel and for bridging large joint gaps.
The Welds have a fine finish and spatter loses are negligible. The
Welding speed is moderate .
Unalloyed Rutil electrodes are not normally recommended for welding
steel having a nominal tensile strength exceeding 440 n/mm.sq.
(45 kg/mm. Sq. ) Rutile electrodes are relatively insensitive to moisture.
High efficiency rutile electrodes generally gives a higher welding speed,
which increases as weld metal recovery increases up to a max . Of About
All are easy to use,give excellent slag detachability, fine bead appearance
and are particularly suitable for welding HORIZONTAL / VERTICAL
FILLETS. The weld metal has tensile properties, which are as high as, or
some what higher then weld metal from unalloyed basic electrodes but
have lower elongation and notch toughness. The evenness of the weld and
the smooth transition to the base metal make joints carried out with Rutile
electrodes at least as good as unmachined joints made with Basic
As regards fatigue strength. Unalloyed Rutile electrodes,irrespective of
their efficiency,can be recommended for welding mild steel having a
nominal tensile strength 440N/mm. Sq.As regards the tensile strength of
the deposit,Rutile electrodes can also be used for welding steel having a
higher nominal tensile strength tan 440 N.mm.sq.,but as a general rule
only electrodes giving LOW HYDROGEN content weld metal, e.g
BASIC,RUTILE- BASIC or ZIRCON- BASIC electrodes should be used
for welding these steels.
Acid electrodes without iron powder in the covering are easier to strike than basic electrodes but more difficult to strike and restrike than rutile
electrodes. The welding speed is moderate.The weld beads are smooth
and shiny. The slag is inflated and easy to remove. The weld metal has a
lower yield stress and tensile strength compared with those from rutile
electrodes but has higher elongation and Impact toughness. This type of
electrodes,which completely dominated the market a few decades ago,has
gradually been replaced by RUTILE electrodes for welding in the flat
position and BASIC electrodes for position welding. Unalloyed acid
electrodes are suitable for welding steels having a nominal tensile
strength of up to 440 N/mm.sq.
High efficiency acid electrodes have considerably higher welding speed then the normal electrodes,up to a maximum of about 120g/min.The
beads are smooth and shiny. The slag is inflated and easy to remove.
High efficiency acid electrodes are particularly suitable for making butt
joints and fillet welds in flat position.
The weld metal has the same strength as that from normal acid
electrodes,and the application range is therefore similar.
Unalloved basic electrodes have moderate welding speed in the flat position but are faster than other type of electrodes when welding
vertically upwards. The reason for this is that basic electrodes can be
deposited at a higher current in the vertical position than other types of
electrodes. In addition the amount of weld metal deposited per electrode
is greater than for other types of electrodes.
The slag is normally not quite as easy to remove as the slag from acid or
rutile type of electrodes,but even so it can be classified as easily
detachable. The slag from basic electrodes has a lower melting point than
that of rutile or acid electrode. The risk of slag inclusions during normal
production welding is therefore unusually small when basic type of
electrodes are used,even if the slag is not completely remoed between
beads during multi-run welding.
The weld metal from basic electrodes has low hydrogen content and
usually good toughness even at low temperatures.Basic electrodes are less
likely to give either HOT CRACKS or COLD CRACKS compared to
other type of electrodes. The superiority of basic electrodes from this
point of view appears when welding manganese alloyed structural
steels,pressure vessel steels and ship plate having a nominal tensile
strengh of 490-530 N/mm.sq. and yield stress of 290-390 N/mm.sq.
Higher the hardenability of steel to be welded,the greater the necessity to
use basic electrodes, and the greater is the need for low covering moisture
Zircon- basic high efficiency electrodes are the fastest of all and are
preferably deposited in the flat position. Zircon basic high efficiency
electrodes can be used for welding the same steels as the unalloyed basic
Rutile-basic high efficiency electrodes combine the good welding
properties of rutile electrodes with high quality weld metal of basic
electrodes. They are therefore the best electrodes for making horizontal vertical fillet welds in high strength steels,where ordinary rutile high
efficiency electrode are not permitted. They can be used for welding the
same steels as ordinary unalloyed basic electrodes or unalloyed zircon-
basic high efficiency electrodes.
Cellulosic electrodes- they are easy to use in all welding positions and
are particularly good for vertical and over head welding. Cellulosic
electrodes are recommended for all position welding where the
mechanical properties of the deposit is of the greatest importance and
radiographic requirements are must to meet. Vertical and over head
welding require often one size larger electrode in comparison to
electrodes with other types of coating. Cellulose electrodes are extremely
good for vertical down welding.
Mild steel can be welded without preheating. Higher tensile steel require
preheating and higher interpass temperature then when the welding is
done with low-hydrogen electrodes.
GUIDE TO ISO CODING
ELECTRODE CLASSIFICATION BY AWS A 5.1
The American Welding Society ( AWS) numbering system can tell a
welder quite a bit about a specific stick electrode including what
application it works best in and how it should be used to maximize
performance. With that in mind ,lets take a look at the system and how it works.The prefix E designates an arc-welding electrode. The first two digits of a 4-digit number and the first three digits of 5 digit number indicate tensile strength. For example,E6010 is a 60,000 psi tensile
strength electrode while E10018 designates a 100,000 psi tensile strength
E 60 1 10 Electrode Tensile strength Position Type of Coating and current
The next to last digit indicates position. The 1 designates an all position electrode, 2 is for flat and horizontal positions only; while 3 indicates an electrode that can be used for flat,horizontal, vertical down and
overhead. The last 2 digits taken together indicate the type of coating and the correct polarity or current to use. See chart below:
Digit Type of coating Welding Current 10 High cellulose sodium Dc +
11 High cellulose potassium Ac or Dc + or Dc -
12 High titania sodium Ac or Dc-
13 High titania potassium Ac or Dc +
14 Iron power titania Ac or Dc- or DC+
15 Low hydrogen sodium DC+
16 Low hydrogen potassium AC or DC+
27 Iron powder iron oxide AC or DC+or DC-
18 Iron powder low hydrogen AC or DC+
20 High iron oxide AC or DC+or DC-
22 High iron oxid AC or DC-
24 Iron powder titania AC or DC- or DC+
28 Low hydrogen potassium iron
AC or DC+
As a welder,there are certain electrodes that you will most likely see and
use time and time again as you go about your daily operations. A DC
machine produces a smoother arc. DC rated electrodes will only run on a
DC welding machin. Electrodes which are rated for AC welding are more
forgiving and can also be used with a DC machin. Here are some of the
most common electrodes and how they are typcally used:
DC only and designed for putting the root bead on the inside of a piece of
pipe,this is the most penetrating arc of all. It is top to dig through rust,
oil,paint or dirt. It is an all-position electrode that beginning welders
usually find extremely difficult,but is loved by pipeline welders world-
This electrode is used for all - position AC welding or for welding on
rusty,dirty,less-than-new metal. It has a deep,penetrating arc and is often
the first choice for repair or maintenance work when DC is unavailable.
This all-position,AC electrode is used for welding clean,new sheet metal.
Its soft arc has minimal spatter,moderate penetration and an easy-to-clean
E 7018 A low- hydrogen,usually DC,all-position electrod